- Text
- Strain,
- Plasticity,
- Gradient,
- Deformation,
- Finite,
- Hwang,
- Classical,
- Cylinder,
- Reference,
- Mesoscale,
- Analysis

Finite deformation analysis of mechanism-based strain gradient ...

248 K.C. Hwang et al. / International Journal **of** Plasticity 19 (2003) 235–251HRR field (Hutchinson, 1968; Rice and Rosengren, 1968). The numerical resultsalso showed that the stress around the crack tip in MSG plasticity is not only moresingular than the HRR field, but also more singular than the classical elastic K field(square-root singularity). This provides a means to explain the cleavage fractureobserved in ductile materials (e.g. Elssner et al., 1994).We use the same loading, material properties, and finite element mesh as Jiang etal. (2001) but the finite **deformation** effect is accounted for. We take a circular domain**of** radius 10 3 l centered at the crack tip in our plane-**strain** finite element **analysis**,where l is the intrinsic material length in (14). The origin **of** the coordinate systemcoincides with the crack tip, while the traction-free crack faces coincide with thenegative x 1 axis. The classical mode-I elastic K field is imposed on the outer boundary**of** the domain (10 3 l) with the elastic stress intensity K I increasing monotonically.The stress intensity factor K I is normalized by Y l 1/2 in the numerical **analysis**,where Y =0.2% E is the initial yield stress, E is the Young’s modulus, and l is theintrinsic material length in (14). The stress is normalized by Y , while the position(coordinate) is normalized by l. Other material properties include the plastic workhardening exponent N=0.2, Poisson’s ratio =0.3, and the reference stress in (13).The empirical material constant in the Taylor dislocation model and the Burgersvector b only appear through the intrinsic material length l in (14), and it is thereforenot necessary to specify the values **of** and b for the above normalizations.Fig 5 shows the distribution **of** the normalized stress ahead **of** the mode-I cracktip, i.e. / Y , versus the normalized distance r/l to the crack tip, where is theCauchy (true) stress along =1.014 ( =180 being the crack faces), and r is thedistance to the crack tip in the reference (undeformed) configuration. The remoteapplied stress intensity factor is K I =10 Y l 1/2 . The distribution **of** for infinitesimal**deformation** MSG plasticity theory (Jiang et al., 2001) and the correspondingcurves for classical plasticity (i.e. without the **strain** **gradient** effect) are also shownfor comparison. For r>10l, all curves become the same straight line with the slope**of** 1/2, corresponding to the elastic K I field (since the slope represents the order **of**singularity in the log–log plot). For r between 0.3l and 10l, all curves still coincidebut they deviate significantly from the straight line (**of** the slope 1/2). This indicatesthat the material undergoes significant plastic **deformation**, though neither the**strain** **gradient** effect nor the finite **deformation** effect is important in this range.Once the distance r to the crack tip is less than 0.3l, the normal stresses predictedby MSG plasticity (for both finite and infinitesimal **deformation**) increase muchquicker than their counterparts in classical plasticity. A representative value **of** theintrinsic material length is l=5 mm [Fleck et al., 1994; Stolken and Evans, 1998; Eq.(14) with =0.5 and b=0.3nm]. At a distance r=0.02l=0.1 mm to the crack tip,which is still within the intended range **of** applications for MSG plasticity (Gao etal., 1999; Huang et al., 2000b), the normal stress predicted by MSG plasticity isapproximately twice **of** that for classical plasticity. For infinitesimal **deformation**theories, the curve for classical plasticity has the slope **of** N/(N+1) and correspondsto the HRR field (Hutchinson, 1968; Rice and Rosengren, 1968), while thecurve for MSG plasticity has the slope higher than 1/2 (in absolute value), indicatingthe crack tip field in MSG plasticity is more singular than not only the HRR field,

K.C. Hwang et al. / International Journal **of** Plasticity 19 (2003) 235–251 249Fig. 5. The Cauchy (true) stress normalized by the initial yield stress Y versus the normalized distanceto the crack tip, r/l, ahead **of** the crack tip (polar angle =1.014 ), where l is the intrinsic materiallength for MSG plasticity, the plastic work hardening exponent N=0.2, Poisson’s ratio =0.3, the ratio**of** yield stress to elastic modulus Y /E=0.2%, and the remotely applied elastic stress intensity factor K I / Y l 1/2 =10. The results are presented for both finite and infinitesimal **deformation** **of** MSG plasticity andclassical plasticity.but also the classical elastic K field. The effect **of** finite **deformation** does not seem tobe significant in Fig. 5, as seen from the comparison between curves for infinitesimaland finite **deformation**. This is because we have taken a relatively small appliedstress intensity factor (K I =10 Y l 1/2 ). In fact, the **strain** is only a few percent (3%)at a distance **of** 0.1 mm (r=0.02l) to the crack tip. It can be established from Fig. 4that the **strain** level needs to be significantly higher (>10%) in order to display thedifference between the finite and infinitesimal **deformation**. We have indeed imposeda much larger applied stress intensity factor, but the finite **deformation** **analysis** hassome numerical difficulties in convergence.6. SummaryWe have developed a finite **deformation** theory **of** **mechanism**-**based** **strain** **gradient**(MSG) plasticity **based** on the Taylor dislocation model. The theory ensuresthe proper decomposition **of** **deformation** into volumetric and deviatoric parts suchthat the volumetric **deformation** does not contribute to the deviatoric **strain** **gradient**,which represents the density **of** geometrically necessary dislocations. We haveconducted the analytic study for a thin cylinder under large torsion, and establishedthat the effect **of** finite **deformation** is significant when R 0 >0.1, where is the twist

- Page 1 and 2: International Journal of Plasticity
- Page 3 and 4: K.C. Hwang et al. / International J
- Page 5 and 6: K.C. Hwang et al. / International J
- Page 7 and 8: K.C. Hwang et al. / International J
- Page 9 and 10: K.C. Hwang et al. / International J
- Page 11 and 12: K.C. Hwang et al. / International J
- Page 13: K.C. Hwang et al. / International J